# Question 6.5: True Stress and True Strain Compare engineering stress and s......

True Stress and True Strain
Compare engineering stress and strain with true stress and strain for the aluminum alloy in Example 6-1 at (a) the maximum load and (b) fracture. The diameter at maximum load is 0.4905 in. and at fracture is 0.398 in.

Step-by-Step
The 'Blue Check Mark' means that this solution was answered by an expert.

Engineering stress S = $\frac{F}{A_{0}}=\frac{8000 \ lb}{(\pi /4)(0.505 \ in.)^2}=39,941 \ psi$

Engineering strain e = $\frac{\Delta l}{l_{0}}=\frac{2.120 \ -­ \ 2.000}{2.000}=0.060 \ in./in.$

True stress = σ = S(1 + e) = 39,941 psi (1 + 0.060) = 42,337 psi
True strain = ln (1 + e) = ln (1 + 0.060) = 0.058 in./in.

The maximum load is the last point at which the expressions used here for true stress and true strain apply. Note that the same answers are obtained for true stress and strain if the instantaneous dimensions are used:

$\sigma=\frac{F}{A}=\frac{8000 \ lb}{(\pi /4)(0.4905 \ in.)^2}=42,337 \ psi$
$\varepsilon =\ln (\frac {A_{0}}{A})=\ln \left[\frac{(\pi /4)(0.505 \ in.)^2}{(\pi /4)(0.4905 \ in.)^2} \right]=0.058 \ in./in.$

Up until the point of necking in a tensile test, the engineering stress is less than the corresponding true stress, and the engineering strain is greater than the corresponding true strain.
(b) At fracture,

$S=\frac{F}{A_{0}}=\frac{7600 \ lb}{(\pi /4)(0.505 \ in.)^2}=37,944 \ psi$
$e=\frac{\Delta l}{l_{0}}=\frac{2.205 \ – \ 2.000}{2.000}=0.103 \ in./in.$
$\sigma =\frac{F}{A_{f}}=\frac{7600 \ lb}{(\pi /4)(0.398 \ in.)^2}=61,088 \ psi$
$\varepsilon = \ln (\frac{A_{0}}{A_{f}} ) = \ln \left[\frac{(\pi /4)(0.505 \ in.)^2}{(\pi /4)(0.398 \ in.)^2} \right]= 0.476 \ in./in.$

It was necessary to use the instantaneous dimensions to calculate the true stress and strain, since failure occurs past the point of necking. After necking, the true strain is greater than the corresponding engineering strain.

Question: 6.7

## Nanoindentation of MgO Figure 6-20 shows the results of an indentation into single crystal (001) MgO using a diamond Berkovich indenter. The unloading stiffness at a maximum indentation depth of 1.45 μm is 1.8 × 10^6 N/m. A calibration on fused silica indicates that the projected contact area at the corresponding contact ...

The projected contact area A_{c}=41 \ \mu m...
Question: 6.6

## Flexural Strength of Composite Materials The flexural strength of a composite material reinforced with glass fibers is 45,000 psi, and the flexural modulus is 18 × 10^6 psi as determined using a three-point bend test. A sample, which is 0.5 in. wide, 0.375 in. high, and 8 in. long, is supported ...

Based on the description of the sample, w = 0.5 in...
Question: 6.1

## Tensile Testing of Aluminum Alloy Convert the load and change in length data in Table 6-1 to engineering stress and strain and plot a stress strain curve. ...

For the 1000-lb load: S=\frac{F}{A_{0}}=\fr...
Question: 6.4

## Ductility of an Aluminum Alloy The aluminum alloy in Example 6-1 has a final length after failure of 2.195 in. and a final diameter of 0.398 in. at the fracture surface. Calculate the ductility of this alloy. ...

% Elongation =  \frac{l_{f} \ - \ l_{0}}{l_...
Question: 6.3

## Young’s Modulus of an Aluminum Alloy Calculate the modulus of elasticity of the aluminum alloy for which the engineering stress strain curve is shown in Figure 6-5. Calculate the length of a bar of initial length 50 in. when a tensile stress of 30,000 psi is applied. ...

When a stress of 34,948 psi is applied, a strain o...
Question: 6.2

## Design of a Suspension Rod An aluminum rod is to withstand an applied force of 45,000 pounds. The engineering stress strain curve for the aluminum alloy to be used is shown in Figure 6-5. To ensure safety, the maximum allowable stress on the rod is limited to 25,000 psi, which is below the yield ...

From the definition of engineering strain, ...